promoting access to White Rose research papers
White Rose Research Online
Universities of Leeds, Sheffield and York
This is a copy of the final published version of a paper published via gold open access
This open access article is distributed under the terms of the Creative Commons
Attribution Licence (
), which permits
unrestricted use, distribution, and reproduction in any medium, provided the
original work is properly cited.
White Rose Research Online URL for this paper:
Sercombe, D, Schwarz, S, Del Pozo-Zamudio, O, Liu, F, Robinson, B.J, Chekhovich,
E.A, Tartakovskii, I.I, Kolosov, O and Tartakovskii, A.I (2013) Optical
Optical investigation of the natural
electron doping in thin MoS
deposited on dielectric substrates
D. Sercombe1, S. Schwarz1, O. Del Pozo-Zamudio1, F. Liu1,2, B. J. Robinson3, E. A. Chekhovich1, I. I. Tartakovskii4, O. Kolosov3& A. I. Tartakovskii1
1Department of Physics and Astronomy, University of Sheffield, Sheffield S3 7RH, United Kingdom,2Experimentelle Physik 2,
Technische Universita¨t Dortmund, 44221 Dortmund, Germany,3Department of Physics, University of Lancaster, Lancaster LA1 4YB,
United Kingdom,4Institute of Solid State Physics, Russian Academy of Sciences, Chernogolovka, 142432, Russia.
Two-dimensional (2D) compounds provide unique building blocks for novel layered devices and hybrid photonic structures. However, large surface-to-volume ratio in thin films enhances the significance of surface interactions and charging effects requiring new understanding. Here we use micro-photoluminescence (PL) and ultrasonic force microscopy to explore the influence of the dielectric environment on optical properties of a few monolayer MoS2films. PL spectra for MoS2films deposited on
SiO2substrates are found to vary widely. This film-to-film variation is suppressed by additional capping of
MoS2with SiO2and SixNy, improving mechanical coupling of MoS2with surrounding dielectrics. We show
that the observed PL non-uniformities are related to strong variation in the local electron charging of MoS2
films. In completely encapsulated films, negative charging is enhanced leading to uniform optical properties. Observed great sensitivity of optical characteristics of 2D films to surface interactions has important implications for optoelectronics applications of layered materials.
Interest in atomically thin two-dimensional (2D) layered compounds is growing due to unique physical properties found for monolayer (ML) structures1,2. One such material, molybdenum disulfide (MoS
generated particular interest due to the presence of an indirect-to-direct band gap transition and observation of photoluminescence (PL)3–5and electro-luminescence6in the visible range up to room temperature. A high on/
off ratio (exceeding 108) has suggested a potential use in field effect transistors7, while a strong valley polarization
is likely to be used in the development of future valleytronics applications8–12.
PL studies4have shown that suspended ML films of MoS
2have enhanced emission compared to those in
contact with the substrate. However, the eventual integration of MoS2into devices, such as transistors and
photonic structures, will render the use of suspended MoS2impractical. The effect of dielectric encapsulation
has so far been reported for high-kdielectric materials commonly used in transistors13–15. However, no thorough
study showing how dielectric environments affect optical properties and charging of MoS2films has yet been
conducted, the two issues we address in this work.
We focus on interaction of MoS2films with SiO2and SixNycommonly used in photonic devices, and report low
temperature PL measurements on over a 100 thin films, enabling detailed insight in interactions of MoS2with its
dielectric surrounding. We study mechanically exfoliated MoS2films deposited on silicon substrates finished with
either nearly atomically flat thermally grown SiO2or relatively rough SiO2grown by plasma-enhanced chemical
vapor deposition (PECVD). We use a combination of low temperature micro-photoluminescence (PL), atomic force microscopy (AFM) and ultrasonic force microscopy (UFM). We find marked variety of the PL spectral lineshapes and peak energies in the large number of few monolayer MoS2films, which nonetheless show trends
that we are able to relate to electrostatic and mechanical interaction of thin films with the surrounding dielectrics. We find that high mechanical coupling between a MoS2film and the surrounding layers is only possible for
capped films on thermally grown SiO2, whereas more complex morphology and poorer contact with the
sur-rounding layers is observed for uncapped films, the effect further exacerbated for films on higher roughness PECVD substrates. Following this observation, we show a direct correlation between the enhanced mechanical coupling of MoS2with the surrounding dielectric layers and increased negative charging of the films, directly
affecting spectral characteristics of PL due to the presence of the pronounced PL peak of a negatively charged
SURFACES, INTERFACES AND THIN FILMS
Received 12 June 2013
Accepted 27 November 2013
Published 12 December 2013
trion. By comparison with recent work where MoS2films were
con-trollably charged by applying voltage16, we estimate that observed
charging lead to electron densities of the order of 1012cm22.
PL of thin MoS2films.We carry out low-temperature PL spectros-copy on a wide range of MoS2films having thicknesses between 2 and
5 ML, as estimated from the careful colour-contrast examination using optical microscopy, and further confirmed for some films from AFM measurement (see Methods for description of sample fabrication and PL techniques). Fig. 1(a) shows a selection of PL spectra measured for uncapped MoS2 films deposited on Si
substrates with either PECVD (a–d) or thermal oxidation (e–h). In all spectra exciton complexesAandBare clearly visible3, although
there is a large variation in PL lineshapes for different films. TheA
complex is composed of a trion PL peak A2 and a high energy
shoulder A0corresponding to neutral exciton PL16. A low energy
shoulderLis also observed in some spectra, though spectra show-ing weak or no contributions ofLandA0states were observed on
both PECVD (a) and thermal oxide (e) substrates. A relatively large contribution of L andA0 was found in many films deposited on
PECVD substrates (b, c) and in some cases the neutral exciton was found to have brighter emission than the trion [as in (d)]. For films deposited on thermal oxide substrates, there is a less significant variation in the lineshape (e–h), and L and A0 features are, in
general, less pronounced relative toA2than in films deposited on
PECVD grown SiO2.
The effect of additional capping of MoS2films with dielectric
layers is demonstrated in Fig. 2. A 100 nm thick layer of either SiO2or SixNyis deposited using PECVD on top of the MoS2/SiO2/
Si samples for both PECVD and thermal SiO2/Si substrates. Here we
observe even less variation in lineshapes between the films. A further suppression of the low energy shoulderLand neutral exciton peakA0
is found for films capped with SixNy(a,b,e,f) on both types of
sub-strates, and with SiO2on thermally grown substrates. In contrast,L
andA0peaks are pronounced when capping with SiO
2is used for
MoS2films on PECVD substrates. Further to this, from comparison
of spectra in (a,b,c,d) and (e,f,g,h), we find that the PL linewidths of
films deposited on the PECVD oxide are notably broader than for those on the thermal oxide substrates.
An interesting trend in all spectra presented in Figs. 1 and 2 is a correlation between the intensities of the featuresLandA0: the two
peaks are either both rather pronounced or suppressed in any given spectrum relative to the trion peakA2. This may imply that peakL
becomes suppressed when the film captures an excess of negative charge.
Analysis of PL peak energies. A statistical analysis of PL peak energies for films deposited on the two types of substrates is presented in Fig. 3. Fig. 3(a,b) show that the average values for the PL peak energies,Eav
max, for uncapped films areEavmax~1:888 eV for
the PECVD substrates and Eavmax~1:880 eV for thermal oxide
substrates, with an almost two times larger standard deviation,
sEmax for the former (18 versus 11 meV). The data collected for
the capped films (shaded for SixNy and hatched for SiO2) are
presented in Fig. 3(c) and (d) for the thermal and PECVD oxide substrates, respectively. Significant narrowing of the peak energy distribution is found in all cases:sEmax<6 meV has been found.
The average peak energies are very similar for both SiO2and SixNy
capping on the thermal oxide substrates (Eavmax~1:874 eV), but differ
for PECVD substrates:Emaxav ~1:862 and 1.870 eV for SiO2and SixNy
From previous reports4, for films with thicknesses in the range 2 to
5 MLs, one can expect the PL peak shift on the order of 20 meV. In addition, PL yield was reported to be about 10 times higher for 2 ML films compared with 4 ML and for 3 ML compared with 5 ML4. In
our study, the integrated PL signal shows a large variation within about one order of magnitude between the films. The dependence of the PL yield on the type of the substrate and capping is not very pronounced. While our data for PL intensities is consistent with the reported in the literature for the range of thicknesses which we studied, the PL peak energy distribution shows the unexpected
Figure 1|PL spectra measured for individual mechanically exfoliated MoS2uncapped films deposited on a 300 nm SiO2layer grown by either
PECVD (a–d) or thermal oxidation (e–h) on a silicon substrate.
Figure 2|PL spectra measured for individual mechanically exfoliated MoS2films capped by a 100 nm PECVD layer of dielectric material.The
effect of capping is shown for films deposited on PECVD grown SiO2 substrates for SixNy(a), (b) and SiO2(c), (d) capping layers, and also for films deposited on thermally grown SiO2and capped with SixNy(e), (f) and SiO2(g), (h).
broadening for uncapped samples: for example, deviations fromEavmax
by620–30 meV are evident in Fig. 3(a,b). For the capped samples, new trends are observed: the significant narrowing and red-shift of
Emaxdistributions. As shown below, these effects reflect changes in
the PL lineshapes between the capped and uncapped samples, which in their turn reflect changes in the relative intensities of theA2,A0
We note that the new experimental trends observed in our PL studies do not depend on the exact distribution of thicknesses in the ensembles of the investigated films, provided these distributions
are similar for all types of samples studied. The latter is the case in our study, as the films were produced using the same method, show similar range of the colour-contrasts under optical examination, and exhibit similar ranges of PL yield.
Analysis of PL lineshapes.In this section we will present the line-shape analysis for theAexciton PL based on the measurement of full width at half maximum (FWHM) in each PL spectrum. This approach allows one to account for contributions of the three PL features,L,A0andA2. The data are summarized in Fig. 4 and Table 1. PECVD grown SiO2substrates.These data are presented in Fig. 4 in
red. Data for uncapped films are shown in Fig. 4(a), from where it is evident that the lineshapes vary dramatically from film to film within a range from 50 to 170 meV. FWHM for uncapped films on PECVD grown substrates is on averageDEFWHMav ~96 with a large standard
deviationsFWHM533 meV. This gives a rather high coefficient of
The non-uniformity of lineshapes of the PL spectra is significantly suppressed by capping the films with SixNyand SiO2(shown with red
in Fig. 4(b) and (c), respectively). This is evidenced from the reduc-tion of the coefficient of variareduc-tion in the FWHM values by a factor of 4 in capped films compared with the uncapped samples (in Table 1). Despite the narrowed spread ofDEFWHMvalues, the average FWHM Figure 3|(a–d) PL peak energies forA exciton complex in MoS2thin films.Data for films deposited on thermally (PECVD) grown SiO2substrates are shown in top (bottom) panels. Panels (a)–(b) and (c)–(d) show PL peak positions for uncapped and capped films, respectively.
Figure 4|PL FWHM of exciton complexA in thin MoS2films.Data for
MoS2films deposited on thermally and PECVD grown SiO2substrates is shown with blue and red, respectively. (a) PL FWHM of uncapped MoS2 films. (b) PL FWHM of SixNycapped MoS2films. (c) PL FWHM of SiO2 capped MoS2films.
Table 1 | Mean values, standard deviations and coefficients of variation for full width at half maximum of PL spectra measured for thin MoS2films
Substrate/Capping Meanvalue Standarddeviation Coefficient ofvariation
PECVD/uncapped 96 meV 33 meV 0.34
PECVD/SiO2 109 meV 9 meV 0.08
PECVD/SixNy 84 meV 7 meV 0.08
Thermal/uncapped 79 meV 12 meV 0.15
Thermal/SiO2 76 meV 7 meV 0.09
in SiO2capped films is rather high, 109 meV, which reflects relatively
strong contribution ofLandA0PL features. Contributions ofA2,L
and A0features vary very considerably in the uncapped samples,
leading to on average smaller linewidths but a very significant spread in FWHM values. In contrast, in SixNycapped films,A2peak
dom-inates and bothLandA0features are relatively weak, which
effec-tively results in narrowing of PL.
Thermally grown SiO2substrates.These data are presented in Fig. 4 in
blue. It can be seen that uncapped films deposited on the flatter thermal oxide substrates appear to have significantly narrower dis-tributions of linewidths compared to uncapped films on PECVD substrates: coefficient of variation of DEFWHM is by a factor of 2
smaller for films on the thermally grown substrates [see Fig. 4(a) and Table 1]. In addition, compared with the films deposited on PECVD grown SiO2, FWHM is also reduced by about 20% to
79 meV. Such narrowing reflects weaker contribution ofLandA0
peaks in PL spectra.
The non-uniformity of the PL spectra still present in uncapped films deposited on thermally grown SiO2is further suppressed by
capping the films with SixNyand SiO2[shown with blue in Fig. 4(b)
and (c), respectively]. In general, the coefficients of variation for FWHM of the capped films are rather similar for both substrates and are in the range of 0.06–0.09, showing significant improvement of the reproducibility of PL features compared with the uncapped samples (see Table 1). For SixNycapped films on thermally grown
SiO2, we also observe narrowing of PL emission to DEavFWHM~
64 meV. This reflects further suppression ofLandA0peaks relative
toA2, the effect less pronounced in SiO
AFM and UFM measurements.To further understand the interac-tions between MoS2films and the substrate/capping materials, we
carried out detailed AFM and UFM measurements of our samples (Fig. 5). AFM measurements of films deposited on PECVD grown substrates Fig. 5(a) show that the film is distorted in shape and follows the morphology of the underlying substrate. The root mean square (rms) roughnessRrmsof these films is 1.7 nm with a
maximum heightRmax511 nm, similar to the parameters of the
substrate,Rrms52 nm andRmax515 nm. SuchRmaxis greater than
the thickness of films (,3 nm), leading to significant film distortions. UFM measurements of these films [Fig. 5(b)] show small areas of higher stiffness (light colour, marked with arrows) and much larger areas of low stiffness (i.e. no contact with the substrate) shown with a dark colour. This shows that the film is largely suspended above the substrate on point contacts.
AFM measurements of films deposited on thermally grown SiO2
substrates [Fig. 5(c)] show a much more uniform film surface due to the less rough underlying substrate. This is reflected in a significantly improvedRrms50.3 nm andRmax51.8 nm. These values are still
higher than those for the bare substrate withRrms50.09 nm and Rmax50.68 nm. A more uniform stiffness distribution is observed
for these films in UFM [Fig. 5(d)], although the darker colour of the film demonstrates that it is much softer than the surrounding sub-strate and thus still has relatively poor contact with the subsub-strate. A darker shading at film edges demonstrates that they have poorer contact than the film center and effectively curl away from the substrate.
AFM and UFM data for films capped with 15 nm SiO2 after
deposition on PECVD and thermally grown SiO2 are given in
Fig. 5(e, f) and (g, h), respectively. For the PECVD substrate, the roughness of the MoS2film is similar to that in the uncapped sample
in Fig. 5(a):Rrms51.68 nm andRmax510.2 nm. From the UFM
data in Fig. 5(f), it is evident that although the contact of the MoS2
film with the surrounding SiO2is greatly improved compared with
the uncapped films, a large degree of non-uniformity is still present, as concluded from many dark spots on the UFM image. In great contrast to that, the capped MoS2film on thermally grown SiO2is
flatter [Fig. 5(g, h)],Rrms50.42 nm andRmax56.1 nm, with the
roughness most likely originating from the PECVD grown SiO2
capping layer. The UFM image in Fig. 5(h) shows remarkable uni-formity of the stiffness of the film similar to that of the capped substrate, demonstrating uniform and firm contact (i.e. improved mechanical coupling) between the MoS2film and the surrounding
There is a marked correlation between the PL properties of the MoS2
films and film stiffness measured by UFM. The stiffness reflects the strength of the mechanical coupling between the adjacent monolayers of the MoS2film and the surrounding dielectrics. The
increased bonding and its uniformity for films deposited on less rough thermally grown SiO2substrates and for capped MoS2films
manifests in the more reproducible PL characteristics, leading to reduced standard deviations of the peak positions and linewidths. These spectral characteristics are influenced by the relative intens-ities of the three dominating PL features, trionA2, neutral excitonA0
and low energyLpeak, which are influenced by the charge balance in the MoS2films sensitive to the dielectric environment. The efficiency
of charging can be qualitatively estimated from the relative intensities ofA2andA0peaks. In the vast majority of the films,A2dominates.
As noted above, the intensity ofA0directly correlates (qualitatively)
with that of the relatively broad low energy PL shoulderL(see Fig. 1 and 2), previously ascribed to emission from surface states. The
line-Figure 5|AFM (left column) and UFM (right column) images for MoS2
thin films deposited on PECVD and thermally grown SiO2substrates.
(a), (b) PECVD substrate, uncapped MoS2film; (c), (d) thermally grown substrate, uncapped MoS2film; (e), (f) PECVD substrate, MoS2film capped with 15 nm of SiO2grown by PECVD; (g), (h) thermally grown substrate, MoS2film capped with 15 nm of SiO2grown by PECVD.
shape analysis presented in Fig. 4 and Table 1 is particularly sensitive to the contribution of peakL.
The PL lineshape analysis and comparison with the UFM data lead to conclusion that negative charging of the MoS2films is relatively
inefficient for partly suspended uncapped films on rough PECVD substrates. Both in SiO2and SixNycapped films on PECVD
sub-strates, the charging effects are more pronounced. However, both
A0andLfeatures still have rather high intensities. The relatively low
charging efficiency is most likely related to a non-uniform bonding between the MoS2 films and the surrounding dielectric layers as
concluded from from UFM data [see Fig. 5(f)]. The charging is more pronounced for uncapped MoS2films on thermal oxide substrates,
and is enhanced significantly more for capped films: for SixNy
cap-pingA0andLpeaks only appear as weak shoulders in PL spectra.
It is clear from this analysis that the charge balance in the MoS2
films is altered strongly when the films are brought in close and uniform contact with the surrounding dielectrics, enabling efficient transfer of charge in a monolithic hybrid heterostructure. Bothn -type4,7,17 andp-type17,18 conductivities have been reported in thin
MoS2films deposited on SiO2. It is thus possible that the sign and
density of charges in exfoliated MoS2films may be strongly affected
by the properties of PECVD grown SiO2and SixNy, where the
elec-tronic properties may vary depending on the growth conditions19–21.
It is notable, however, that for a large variety of samples studied in this work, the negative charge accumulation in the MoS2films is
pronounced, and is further enhanced when the bonding of the films with the dielectric layers is improved.
In order to estimate the density of the accumulated charges we refer to Ref. 16, where PL spectra as a function of electron density in the film were measured. The neutral exciton PL peakA0becomes less
intense than the trion peak A2 at the electron densityn <23
1012cm22. Since in our experiments in many filmsA0peak is
rela-tively pronounced, we conclude that we have studied the regime where the electron densities are of the order of 1012cm22or less.
The band-structure of MoS2and hence its optical characteristics
can also be influenced by strain22–24. However, the distribution and
magnitude of strain cannot be assessed directly in our experiments. Indirect evidence for increased tensile strain in capped samples com-pared to uncapped films on PECVD may be deduced from the red-shift of the average PL peak energy by,20 meV after capping (data in Fig. 3). On the other hand, doping-dependent Stokes shifts of the trion PL have been found recently16, which may explain the behavior
we find in charged MoS2sheets. One would expect a more uniform
strain distribution in the case of uniform mechanical properties of the sample, which as shown by UFM is achieved for capped MoS2
films on flat thermally grown SiO2substrates. In order to roughly
estimate a possible magnitude of strain in our films we refer to recent work in Refs. 24–26 reporting 50 to 80 meV bandgap shift per per-cent of applied strain. This implies that in our experiments the max-imum strain in the films reaches<0.5%.
We note, that another method for sensing the strain and charging in thin MoS2films is by using Raman spectroscopy. Recently it has
been found that Raman modes27E1
2gandA1gexhibit frequency shifts
under the influence of strain25,26,28 and charging29. We have also
carried out preliminary Raman experiments on a set of films placed on PECVD and thermally grown SiO2substrates and capped with
SiO2and SixNy. However, only very weak trends have been observed.
This is consistent with relatively low charging densities and strain in our samples, the effect of which is readily detectable in PL16,25,26, but is
less pronounced in Raman measurements.
In conclusion, we demonstrate that it is possible to increase the reproducibility of optical characteristics of mechanically exfoliated few mono-layer MoS2 films by coating the films with additional
dielectric layers of either SiO2or SixNy. By comparing PL data with
results obtained in UFM, we show that there is a direct correlation between the degree of the mechanical coupling of the MoS2films to
the surrounding dielectrics and uniformity of the optical properties. We show that a wide spread in PL spectral lineshapes occurs in general as a result of the film-to-film variation of the relative intens-ities of the negatively charged trion peak A2 and the two other
features, neutral exciton peakA0and a low energy PL bandL. We
find that when the mechanical coupling between the films and the dielectrics is improved, the films become increasingly negatively charged, as deduced from the pronounced increase in PL of the trion peak, dominating in the majority of PL spectra. Such charging, and also possibly reduction in strain non-uniformities, underpins the highly uniform PL properties in capped MoS2films, leading to the
smallest linewidths below 70 meV for thin MoS2films deposited on
thermally grown SiO2and capped with a SixNylayer.
Note: Since this work has been submitted, two more detailed stud-ies of interaction of MoS2 films with substrates have become
Sample preparation.MoS2was exfoliated using the mechanical cleavage method1
and deposited on commercially purchased Si wafers with a low roughness 300 nm thick thermally grown SiO232. Further MoS2samples were produced using the same
technique, but deposited on Si substrates covered with 300 nm PECVD grown SiO2.
PECVD deposition was done in a 60uC chamber with a sample temperature of 300uC. The root mean square (rms) roughness,Rrms, of the PECVD grown SiO2is found to be
2 nm with a maximum peak height of 15 nm, whereasRrmsof the thermally grown
SiO2is 0.09 nm with a maximum height of 0.68 nm. The additional capping of the
MoS2/SiO2/Si samples with SixNyand SiO2was carried out using the same PECVD
techniques. The complete SiO2/MoS2/SiO2/Si or SixNy/MoS2/SiO2/Si samples had the
top SixNyand SiO2layers with thicknesses of 100 nm for PL and 15 nm for AFM/
UFM measurements. The high surface roughness rendered impractical use of AFM for measurements of the film thicknesses on PECVD substrates. However, independent of the substrate type, the uncapped thin MoS2films had optical contrasts
corresponding to thicknesses of 2–5 MLs, further confirmed by AFM on thermal oxide substrates. Furthermore, the range of PL yield was similar for all four types of sample independent of the substrate and capping type, further indicating that ensembles of films with similar distributions of film thicknesses were measured.
Micro-photoluminescence experiments.Low temperature (10 K) micro-PL was carried out on a large number of thin films in a continuous flow He cryostat. The signal was collected and analyzed using a single spectrometer and a nitrogen-cooled charged-coupled device. The sample was excited with a laser at 532 nm. All PL spectra presented in this work were measured in a range of low powers where no dependence on power of PL lineshape was found.
AFM/UFM experiments.As shown elsewhere33, the ultrasonic force microscopy
(UFM) allows imaging of the near-surface features and subsurface interfaces with superior nanometre scale resolution compared to AFM techniques34. In the
sample-UFM modality used in this paper35, the sample in contact with the AFM tip is vibrated
at small amplitude (0.5–2 nm) and high frequency (2–10 MHz), much higher than the resonance frequencies of the AFM cantilever. The resulting sample stress produces a reaction, that is modified by the voids, subsurface defects or sample-substrate interfaces, and can be detected as an additional ‘ultrasonic’ force. A unique feature of UFM is that it enables nanometre scale resolution imaging of morphology of subsurface nano-structures and interfaces of solid-state objects. In order to interpret the images of a few layer films presented in Fig. 5, one can note that the bright (dark) colors correspond to higher (lower) sample stiffness.
1. Novoselov, K. S.et al. Two-dimensional atomic crystals.PNAS102, 10451–10453 (2005).
2. Wang, Q. H., Kalantar-Zadeh, K., Kis, A., Coleman, J. N. & Strano, M. S. Electronics and optoelectronics of two-dimensional transition metal dichalcogenides.Nature Nanotechnology7, 699–712 (2012).
3. Splendiani, A.et al. Emerging Photoluminescence in Monolayer MoS2.Nano
Letters10, 1271–1275 (2010).
4. Mak, K., Lee, C., Hone, J., Shan, J. & Heinz, T. Atomically Thin MoS2: A New
Direct-Gap Semiconductor.Phys. Rev. Lett.105, 136805 (2010).
5. Eda, G.et al. Photoluminescence from Chemically Exfoliated MoS2.Nano Letters
11, 5111–5116 (2011).
6. Sundaram, R. S.et al. Electroluminescence in Single Layer MoS2.Nano Letters13,
7. Radisavljevic, B., Radenovic, a., Brivio, J., Giacometti, V. & Kis, A. Single-layer MoS2transistors.Nature Nanotechnology6, 147–150 (2011).
8. Mak, K. F., He, K., Shan, J. & Heinz, T. F. Control of valley polarization in monolayer MoS2by optical helicity.Nature Nanotechnology7, 494–498 (2012).
9. Sallen, G.et al. Robust optical emission polarization in MoS2monolayers through
10. Zeng, H., Dai, J., Yao, W., Xiao, D. & Cui, X. Valley polarization in MoS2
monolayers by optical pumping.Nature Nanotechnology7, 490–493 (2012). 11. Cao, T.et al. Valley-selective circular dichroism of monolayer molybdenum
disulphide.Nature Communications3, 887 (2012).
12. Xiao, D., Liu, G.-B., Feng, W., Xu, X. & Yao, W. Coupled Spin and Valley Physics in Monolayers of MoS2and Other Group-VI Dichalcogenides.Phys. Rev. Lett.
108, 196802 (2012).
13. Jena, D. & Konar, A. Enhancement of Carrier Mobility in Semiconductor Nanostructures by Dielectric Engineering.Phys. Rev. Lett.98, 136805 (2007). 14. Plechinger, G.et al. Low-temperature photoluminescence of oxide-covered
single-layer MoS2.Phys. Status Solidi RRL6, 126–128 (2012).
15. Yan, R.et al. Raman and Photoluminescence Study of Dielectric and Thermal Effects on Atomically Thin MoS2.arXiv:1211.4136v1 [cond-mat.mtrl-sci](2012).
16. Mak, K. F.et al. Tightly bound trions in monolayer MoS2.Nature Materials11,
17. Dolui, K., Rungger, I. & Sanvito, S. Origin of the n-type and p-type conductivity of MoS2monolayers on a SiO2substrate.Phys. Rev. B87, 165402 (2013).
18. Zhan, Y., Liu, Z., Najmaei, S., Ajayan, P. M. & Lou, J. Large-Area Vapor-Phase Growth and Characterization of MoS2Atomic Layers on a SiO2Substrate.Small8,
19. De Wolf, S., Agostinelli, G., Beaucarne, G. & Vitanov, P. Influence of stoichiometry of direct plasma-enhanced chemical vapor deposited films and silicon substrate surface roughness on surface passivation.J. of Appl. Phys.97, 063303 (2005).
20. Boogaard, A., Kovalgin, A. & Wolters, R. Net negative charge in low-temperature SiO2gate dielectric layers.Microelectronic Engineering86, 1707–1710 (2009).
21. Zou, X. & Zhang, J. Study on PECVD SiO2/Si3N4double-layer electrets with
different thicknesses.Science China Technological Sciences54, 2123–2129 (2011). 22. Peelaers, H. & Van de Walle, C. G. Effects of strain on band structure and effective
masses in MoS2.Phys. Rev. B86, 241401 (2012).
23. Conley, H. J.et al. Bandgap Engineering of Strained Monolayer and Bilayer MoS2.
24. He, K., Poole, C., Mak, K. F. & Shan, J. Experimental demonstration of continuous electronic structure tuning via strain in atomically thin MoS2.arXiv:1305.3673
25. Castellanos-Gomez, A.et al. Local Strain Engineering in Atomically Thin MoS2.
Nano Letters; DOI:10.1021/nl402875m (2013).
26. Zhu, C. R.et al. Strain tuning of optical emission energy and polarization in monolayer and bilayer MoS2.Phys. Rev. B88, 121301(R) (2013).
27. Zhang, X.et al. Raman spectroscopy of shear and layer breathing modes in multilayer MoS2.Phys. Rev. B87, 115413 (2013).
28. Rice, C.et al. Raman-scattering measurements and first-principles calculations of strain-induced phonon shifts in monolayer MoS2.Phys. Rev. B87, 081307 (R)
29. Chakraborty, B.et al. Symmetry-dependent phonon renormalization in monolayer MoS2transistor.Phys. Rev. B85, 161403(R) (2012).
30. Buscema, M., Steele, G. A., van der Zant, H. S. J. & Castellanos-Gomez, A. The effect of the substrate on the Raman and photoluminescence emission of single layer MoS2. arXiv:1311.3869 [cond-mat.mtrl-sci] (2013).
31. Scheuschner, N.et al. Photoluminescence of freestanding single- and few-layer MoS2. arXiv:1311.5824 [cond-mat.mtrl-sci] (2013).
32. Benameur, M. M.et al. Visibility of dichalcogenide nanolayers.Nanotechnology 22, 125706 (2011).
33. Kolosov, O. & Yamanaka, K. Nonlinear Detection of Ultrasonic Vibrations in an Atomic Force Microscope.Jpn. J. Appl. Phys.7(1993).
34. Yamanaka, K., Ogiso, H. & Kolosov, O. Analysis of Subsurface Imaging and Effect of Contact Elasticity in the Ultrasonic Force Microscope.Appl. Phys. Lett.64, 178 (1994).
35. McGuigan, A. P.et al. Measurement of debonding in cracked nanocomposite films by ultrasonic force microscopy.Appl. Phys. Lett.80, 1180 (2002).
This work has been supported by the Marie Curie ITNs S3NANO and Spin-Optronics,
EPSRC Programme grant EP/J007544/1, and EU FP7 GRENADA grant. O. D. P.-Z. thanks CONACYT-Mexico Doctoral Scholarship.
D.S. and S.S. made the samples. D.S., S.S., O.D.P.-Z., F.L., I.I.T. and E.A.C. measured and analyzed optics data. B.J.R. and O.K. measured AFM and UFM. D.S. and A.I.T. wrote the manuscript with input from all co-authors. E.A.C. supervised optical spectroscopy experiments. A.I.T. guided the project.
Competing financial interests:The authors declare no competing financial interests.
How to cite this article:Sercombe, D.et al. Optical investigation of the natural electron doping in thin MoS2films deposited on dielectric substrates.Sci. Rep.3, 3489; DOI:10.1038/
This work is licensed under a Creative Commons Attribution 3.0 Unported license. To view a copy of this license, visit http://creativecommons.org/licenses/by/3.0